**Modelling of Gas Tungsten Arc Welding Pool under **

**Marangoni Convection **

**Steven Wang, Roy Nates, Timotius Pasang, Maziar Ramezani**

*****

Department of Mechanical Engineering, Auckland University of Technology, New Zealand

Copyright © 2015 by authors, all rights reserved. Authors agree that this article remains permanently open access under the terms of the Creative Commons Attribution License 4.0 International License

**Abstract**

**Due to lack of comprehensive experimental**

studies on welding processes, and to better understand the mechanisms behind these processes, especially the weld pool shape variations suspected due to Marangoni Effect or surface tension shear stress, a two-dimensional simulation model was developed to study the physics of gas tungsten arc welding (GTAW). Experimental spot-welds on Ti-5Al-5Mo-5V-3Cr was carried out to compare to the model for crucial clues such as, the magnitude of Marangoni convectional stress that is difficult to determine experimentally; and to estimate the Enhancement Factor, an artificial parameter incorporated into the model proven to account for any discrepancies between simulated results and experimental weld pool shapes, due to lack of viscosity temperature dependent data as well as flow instabilities. The model confirmed that Marangoni Convection is indeed the most dominant force in shaping the weld pool, followed by thermal buoyancy force and electromagnetic force. As the investigation went on, the validity of past welding simulations assuming a constant flow scheme was examined, concluding with the recommendation of applying a laminar flow regime at the initial welding times and turbulent flow with elapsing welding time to effectively eliminate simulation inaccuracies.

**Keywords**

*Fluent, GTAW, Marangoni Convection,*

Simulation, Welding

**1. Introduction **

With several different fusion welding processes, the melted weld pool profile which ultimately solidifies to form the fusion zone, diverging greatly by a wide variety of factors, e.g. base material, workpiece size, machine setups and extensive range of other process variables. For each distinctive welding setup, the weld pool geometry could vary considerably, and thought to be largely dependent on the hydrodynamics of the weld pools [1].

During the last couple of decades, the weld pool

characteristics were broadly studied, these included experimental studies and more recently numerical studies involving CFD simulations.

Experimental studies on weld pool behaviours were
largely focused on the flow characteristics, but were rather
limited due to difficulty that light could not travel through
liquid metal or poor opacity, not to mention the tight space as
weld pools are generally in the order of millimetres, coupled
with extremely high temperature nature of the welding
processes, all made measuring the flow near impossible.
Reported researches in the area of Marangoni convection
were essentially owed to the validation of the ability of
surface active elements within the workpiece to modify the
flow pattern [2], allowing some understanding of the internal
flow characteristics of the weld pool. Into the 21st_{ century, }
experimental studies were taken to the next level with the
assistance of X-ray transmission devices, the internal flow
could now be accurately captured in motion and examined in
detail [3].

As for numerical studies, given the rapid development of CFD software packages, modern welding researchers could now be able to simulate welding processes with nearly unlimited possibilities, taking into account the flow regime e.g. laminar or turbulent, modelling the solidification stage, sensitivity analysis on wide variety of operating parameters, effect of shielding gas and so on. Overall, previous numerical studies could be divided into the following assumption/basis groups: 2D or 3D, free or flat surface, incorporation of solidification stage and laminar or turbulent flow. As for the model orientation, 2D and 3D models did not deviate much in terms of capabilities to perform enormous range of studies on the weld pool behaviours, and showed identical results,

plasma direct metal forming process. The model revealed that the velosity of the front part of the pool is a little slower than aft part. Marangoni convection reinforced the convection and enhanced the heat transfer. Sandor et al. [6] showed that a thin layer of silica flux leads to an increased depth of weld penetration during activated TIG welding of Armco iron. The oxygen-content is found higher in the solidified weld metal and it was linked to the increased depth of penetration through the reversed Marangoni convection. It was theoretically shown for the first time that the basic reason of the reversed Marangoni convection is the phenomenon called “surface phase transition”, leading to the formation of a nano-thin FeO layer on the surface of liquid iron.

With the above information in mind, the debate on 2D or 3D, free or flat surface and incorporation of solidification would be settled; there would be little difference in terms of result accuracy [7]. Whereas, as for the flow regime, almost all welding researches had either applied laminar flow regime or turbulent flow assumption both with enhancement factors to account for under calculations of momentum and energy, in order to get good agreements with experimental results [8].

This research group believe that Marangoni Effect is the dominant force in weld pool shaping; also that the “constant” laminar or turbulent flow assumption would be fundamentally flawed, since fluid flow should not be consistently laminar or turbulent all the way through as done

by past numerical studies; and to better understand the weld pool behaviours, a two-dimensional simulation model was constructed in Fluent® based on stationary arc GTAW welding conditions. In addition, GTAW welding experiments were also performed on titanium alloy Ti-5Al-5V-5Mo-3Cr as reference data for the numerical results validation.

**1.1. Marangoni Convection in Weld Pools **
**Marangoni Effect **

The Marangoni Effect or thermo-capillary effect, is the effect of mass transfer of fluids due to surface tension gradient; it was first identified by physicist James Thomson in 1855, by the phenomenon “tears of wine” [9]. Not long after the discovery, the Italian Physicist Carlo Marangoni studied this phenomenon in his doctoral thesis and was published in 1865; the general physical effect is then name after him [10].

The concluding remark was that liquid with higher surface tension would pull more strongly on the surrounding liquid than the one with lower surface tension, since water has a higher surface tension than alcohol, this surface tension gradient would cause the liquid to flow away from regions of lower surface tension (the alcohol) [10]; hence as observed, water is convectively and naturally flowing outward to the glass.

**Figure 2**. Photo of tears of wine and illustration of Marangoni Effect

**Marangoni Number **

The Marangoni number is a dimensionless number describing the relative importance of surface tension forces to viscous forces [9]. It is illustrated in the following form:

𝑴𝑴𝑴𝑴=−𝒅𝒅𝒅𝒅_{𝒅𝒅𝒅𝒅}∙𝑳𝑳∆𝒅𝒅_{𝝁𝝁𝝁𝝁} (1)
where 𝛾𝛾 is the surface tension stress, *T* the temperature of
the weld pool, *L* the characteristic length, 𝛼𝛼 the thermal
diffusivity of the workpiece, and 𝜇𝜇 the dynamic viscosity of
the material.

This number was established in an attempt to evaluate and
quantify the Marangoni Effect, mostly used in mass transfer
applications such as dopant distribution in silicon fibres and
semi-conductors [9]; as for welding applications, the more
relevant surface tension temperature gradient, the 𝑑𝑑𝛾𝛾 𝑑𝑑𝑇𝑇⁄
term is of great importance, values can range from negative
to positive. Although the values for the surface tension
temperature gradient are somewhat exceedingly small,
usually in the order of ±5 × 10−4_{𝑁𝑁}_{/}_{𝑚𝑚 ∙ 𝐾𝐾}_{, whereas this }
decimal number along with the sign change would have
crucial implications to the weld pool geometry because of

the very distinctive flow behaviours [11].
**Surface Tension Temperature Gradient **

As mentioned before, the weld pool shape is believed to be
very dependent on *Marangoni* convection, in the centre of it
all, is the surface tension temperature gradient. For welding
processes, the workpiece would contain some degree of
impurities, such as oxygen and sulphur found in steels;
during welding, these impurities were discovered to be very
‘surface active’, altering the surface tension gradient
together with temperature, thus making the term extremely
complex to formulate [12].

To make things simpler and easier to comprehend, as a general trend, the surface tension temperature gradient would be altered by the amount of surface active elements present along with a critical temperature to change the sign of 𝑑𝑑𝛾𝛾 𝑑𝑑𝑇𝑇⁄ , resulting in three scenarios of convective fluid flow [13]:

**Figure 3.** Wide and shallow pool by negative gradient

This would lead to the surface temperature greater than the critical temperature, thus surface tension is lower in the high temperature region, the pool centre; therefore according to Marangoni convection theories, liquid metal would experience an outward flow from the pool centre.

(2) 𝒅𝒅𝒅𝒅 𝒅𝒅𝒅𝒅⁄ can be both positive and negative across the pool when surface active element concentration is increased;

**Figure 4. **"W" shaped pool by pool boundary not yet surpassing the critical temperature

Under this scenario, the critical temperature sits in between the pool centre and boundary, inducing a zero 𝑑𝑑𝛾𝛾 𝑑𝑑𝑇𝑇⁄ in the pool at this temperature where the surface tension is highest. So as the temperature at the pool centre would be higher than the critical temperature, a negative 𝑑𝑑𝛾𝛾 𝑑𝑑𝑇𝑇⁄ would be initiated, thus outward flow; likewise at the pool edge, its temperature (melting point) would be lower than the critical temperature, a positive 𝑑𝑑𝛾𝛾 𝑑𝑑𝑇𝑇⁄ would be encouraged, hence inward flow. By combining these two distinctive flow patterns, a “W” or “dog-bone” shaped pool would be created.

(3) Positive 𝒅𝒅𝒅𝒅 𝒅𝒅𝒅𝒅⁄ when surface active element concentration is further increased;

**Figure 5.** Deep and narrow pool by positive gradient

**1.2. Forces in GTAW **
**Surface Tension Force **

As discussed previously, surface tension force, or Marangoni convection does play an exceptional role in weld pool formation. Even though this critical temperature is vastly unknown for most materials, but with the absence of surface active elements, the surface tension temperature gradient would be negative for most materials [13]. In other words, wide and shallow pool shapes would be observed for most materials because a negative gradient would induce outward flow patterns from the pool centre to the pool edge; hence the surface temperature had typically fully surpassed the critical temperature for outward flow.

However with the surface active elements into the equation, things do get a lot more complicated; the weld pool fluid flow would be altered dramatically with addition of surface active elements into the material, as well as changing concentration of the surface active element [13].

As suggested by Limmaneevichitr and Kou [14] in their experimental work, by adding surface active element of C2H5COOK while keeping all other process parameters constant, the surface tension temperature gradient of NaNO3 changed from negative to positive, and so did the flow pattern from outward to inward. Essentially, their studies on the surface active elements and weld pool behaviour were based on one significant work produced by Sahoo et al. [15] where they had given the issue a mathematical treatment as following:

𝒅𝒅𝒅𝒅 𝒅𝒅𝒅𝒅=

𝒅𝒅𝒅𝒅

𝒅𝒅𝒅𝒅�𝒐𝒐− 𝑹𝑹𝚪𝚪𝑺𝑺𝐥𝐥𝐥𝐥(𝟏𝟏+𝑲𝑲𝑴𝑴𝒊𝒊)
−_{(}_{𝟏𝟏}_{+}𝑲𝑲𝑴𝑴_{𝑲𝑲𝑴𝑴}𝒊𝒊

𝒊𝒊)

𝚪𝚪𝑺𝑺�∆𝑯𝑯𝒐𝒐− ∆𝑯𝑯�𝒊𝒊𝑴𝑴� 𝒅𝒅

𝑲𝑲=𝒌𝒌𝟏𝟏𝒆𝒆𝒆𝒆𝒆𝒆 �−∆𝑯𝑯

𝒐𝒐

𝑹𝑹𝒅𝒅 � (2)
where 𝑑𝑑𝛾𝛾/𝑑𝑑𝑇𝑇|𝑜𝑜 denotes surface tension temperature
gradient for pure metal, *R* gas constant, ΓS surface excess at
concentration, ∆𝐻𝐻𝑜𝑜 _{ standard heat of absorption, ∆𝐻𝐻�}

𝑖𝑖𝑀𝑀 partial molar enthalpy of species mixing in the solution, 𝑘𝑘1 constant to entropy of segregation and 𝑎𝑎𝑖𝑖 activity of the element in material.

By having this mathematical model, it does give welding researchers some insights into ways of surface active elements in influencing the surface tension force, hence weld pool fluid flow and ultimately the pool geometry.

However, it is only useful in determining the surface tension temperature gradient for one active element at a time; this would obviously be the major drawback of this approximation. For instance commonly for steels, two main active elements would be present, oxygen and sulphur, but only one element could be assessed each time, and the other element would be ignored. This is mainly why most welding researches would only use constant surface tension temperature gradient values, also because that there are just so many things happening at once during the weld pool formation.

**Electromagnetic Force **

For a GTAW process, electromagnetic force would be present. Since electric current is flowing through the conductor (workpiece), a magnetic field would be produced; as a result the liquid weld pool would be subject to this induced magnetic field, causing convective flow. Generally the flow direction would be inward referring to Kou & Sun and their findings [16].

**Figure 6. ** Schematic diagram of electromagnetic force acting in the
GTAW weld pool (left); inward flow pattern (right); redrawn from Kou [17]

The electromagnetic force 𝐹𝐹⃗𝑒𝑒𝑒𝑒 or Lorentz force, is governed by the equation below:

𝑭𝑭��⃗𝒆𝒆𝒆𝒆=𝑱𝑱⃗×𝑩𝑩��⃗ (3) where 𝐽𝐽⃗ and 𝐵𝐵�⃗ are the current density vector and magnetic flux vector in the weld pool respectively.

Early studies of Kou and Sun [16] saw the development of a set of equations to accurately simulate the electromagnetic force with the aid of Maxwell’s equations in reference to the Magneto-hydrodynamics approximation, for a three-dimensional axis-symmetric welding system under spot welding (stationary arc) conditions. The simulation was done for thick aluminium alloy AA6061 plate, for a current of 150 A, voltage of 15 V and an assumed efficiency of 80%, returned a 25 cm/s maximum velocity in the weld pool. Thus the electromagnetic force would be considered quite significant in terms of magnitude in the weld pool.

Further studies were done by Kumar and DebRoy [18] in an attempt to accurately model the electromagnetic force in a GTAW weld pool, where considerations of base metal geometry, arc distance to workpiece, electrode current, arc plasma, current distribution were all taken into account; again the simulation was done for three-dimensional, axis-symmetric systems.

As for two-dimensional modelling of electromagnetic force in a weld pool, Shi et al. [19] applied the following equations by considering the forces separately in both axial and radial directions:

**Axial Direction **

𝑬𝑬𝑴𝑴𝒛𝒛= 𝝁𝝁𝒆𝒆𝑰𝑰

𝟐𝟐

𝟒𝟒𝝅𝝅𝟐𝟐_{𝒓𝒓}𝟐𝟐_{𝒛𝒛}_{𝑳𝑳}�(𝟏𝟏 − 𝐞𝐞𝐞𝐞𝐞𝐞�−

𝒓𝒓𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐��

𝟐𝟐
�_{𝒛𝒛}𝒛𝒛

**Radial Direction **

𝑬𝑬𝑴𝑴𝒓𝒓= 𝝁𝝁𝒆𝒆𝑰𝑰

𝟐𝟐

𝟒𝟒𝝅𝝅𝟐𝟐_{𝝈𝝈}_{𝒋𝒋}𝟐𝟐𝒆𝒆𝒆𝒆𝒆𝒆 �− 𝒓𝒓
𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐� �(𝟏𝟏 − 𝐞𝐞𝐞𝐞𝐞𝐞�−

𝒓𝒓𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐�� �

𝒛𝒛 𝒛𝒛𝑳𝑳�

𝟐𝟐 (5) where 𝜇𝜇𝑒𝑒 is the magnetic permeability, 𝐼𝐼 the welding current, 𝑧𝑧𝐿𝐿 thickness of the workpiece, 𝜎𝜎𝑗𝑗 effective current distribution parameter, 𝑟𝑟 and 𝑧𝑧 the radial and axial distance respectively.

**Buoyancy Force **

For any weld pool, the temperature in the pool centre would be higher than the temperature found at the pool boundary; and since the density of the liquid metal at a higher temperature would be lower, then as illustrated in Fig. 7, an upward buoyancy force would be created as at Point a; as for Point b near the pool boundary, where the temperature would be considerably lower than at Point a, a downward force would be expected [20].

**Figure 7.** Schematic diagram of buoyancy force acting on the weld pool
(left); density difference between point a and b (middle); outward flow
(right). Redrawn from Kou [20]

The upward forces at the hotter regions coupled with downward force at the cooler regions would inevitably produce a convective shift of liquid metal originating from the centre to the pool edge, causing an outward flow situation as seen in Fig. 7 (right).

Buoyancy force could be calculated by Boussinesq approximation [21]:

𝑩𝑩=−𝝆𝝆𝝆𝝆𝝆𝝆(𝒅𝒅 − 𝒅𝒅𝒐𝒐) (6)
where 𝜌𝜌 is the density of the liquid metal, 𝑔𝑔 the
gravitational acceleration constant, 𝛽𝛽 thermal expansion
coefficient, 𝑇𝑇 temperature of liquid metal and 𝑇𝑇𝑜𝑜 reference
temperature which is normally the room temperature.
**ARC Plasma Force **

The arc plasma shear stress exists by the simple fact that the arc plasma contains kinetic energy as well as momentum [22]. When the arc plasma strikes the weld pool at the pool centre, an outward shear force would be exerted on the pool surface as shown in Fig. 8 (left). Similar to surface tension forces, this shear stress initiated from the pool surface would certainly drive outward convective flow of liquid metal as indicated in Fig 8 (right).

In most cases, the magnitude of the force generated by arc plasma would be the least significant amongst surface tension force, electromagnetic force and buoyancy force [23]. However, according to the study conducted by Matsunawa and Yokoya [24], the arc plasma force may be substantially increased for a long arc length (8 – 10 mm) welding process, as well as with excessively high welding current since the

momentum and kinetic energy level would be raised drastically.

**Figure 8. ** Schematic diagram of buoyancy force acting on the weld pool
(left); density difference between point a and b (middle); outward flow
(right). Redrawn from Kou [20]

**2. Numerical Modelling **

**2.1. Assumptions Made **

In numerical study conducted in this paper, the following assumptions were made:

(1). Two-dimensional transient heat transfer process (2). Flat surface with no surface deformations;

(3). Standard k-ε turbulent model (laminar flow also investigated);

(4). Fluid as incompressible Newtonian; (5). Axisymmetric along the z-axis;

(6). Gas phase ignored (only solid and liquid phases); (7). Gaussian distribution of the heat flux;

(8). Approximate change of latent heat of melting for materials as linear;

(9). Arc plasma force small enough to be ignored (low current level and short arc welding processes); (10).Ambient temperature as 300 K

(11).Ambient pressure at 101.325 kPa

**2.2. Governing Conservation Equations **

Confining to the above assumptions, the conservation equations resulting in the following forms [25]:

**Conservation of Mass **
𝟏𝟏
𝒓𝒓

𝝏𝝏(𝒓𝒓𝒓𝒓) 𝝏𝝏𝒓𝒓 +

𝝏𝝏𝝏𝝏

𝝏𝝏𝒛𝒛=𝟎𝟎 (7)
**Conservation of Momentum in Axial Direction **

𝝆𝝆 �𝝏𝝏𝝏𝝏_{𝝏𝝏𝝏𝝏}+𝒓𝒓𝝏𝝏𝝏𝝏_{𝝏𝝏𝒓𝒓}+𝝏𝝏𝝏𝝏𝝏𝝏_{𝝏𝝏𝒛𝒛}�=−𝝏𝝏𝒆𝒆_{𝝏𝝏𝒛𝒛}+𝝁𝝁 �𝝏𝝏_{𝝏𝝏𝒓𝒓}𝟐𝟐𝝏𝝏𝟐𝟐+

𝝏𝝏𝝏𝝏 𝒓𝒓𝝏𝝏𝒓𝒓+

𝝏𝝏𝟐𝟐_{𝝏𝝏}

𝝏𝝏𝒛𝒛𝟐𝟐�+𝑺𝑺𝒛𝒛 (8)

**Conservation of Momentum in Radial Direction **
𝝆𝝆 �𝝏𝝏𝒓𝒓_{𝝏𝝏𝝏𝝏}+𝒓𝒓𝝏𝝏𝒓𝒓_{𝝏𝝏𝒓𝒓}+𝝏𝝏𝝏𝝏𝒓𝒓_{𝝏𝝏𝒛𝒛}�=−𝝏𝝏𝒆𝒆_{𝝏𝝏𝒓𝒓}+𝝁𝝁 �𝝏𝝏_{𝝏𝝏𝒓𝒓}𝟐𝟐𝒓𝒓𝟐𝟐+

𝝏𝝏𝒓𝒓 𝒓𝒓𝝏𝝏𝒓𝒓−

𝒓𝒓 𝒓𝒓𝟐𝟐+

𝝏𝝏𝟐𝟐_{𝒓𝒓}

𝝏𝝏𝒛𝒛𝟐𝟐�+𝑺𝑺𝒓𝒓

(9)
**Conservation of Energy **

where 𝑧𝑧, 𝑟𝑟, 𝑢𝑢, 𝑣𝑣, 𝜌𝜌, 𝑝𝑝, 𝜇𝜇, 𝑘𝑘, 𝑇𝑇 and 𝐶𝐶𝑝𝑝 are the axial distance, radial distance, radial velocity, axial velocity, density of material, pressure, viscosity of liquid metal, thermal conductivity, temperature of liquid metal, and specific heat respectively. In addition, 𝑆𝑆𝑧𝑧 and 𝑆𝑆𝑟𝑟 are the non-standard momentum source terms in the axial and radial direction, topped with 𝑆𝑆𝑒𝑒 the energy source term.

**2.3. Momentum & Energy Source Terms **
**Axial Momentum Source & Sink Term **

𝑺𝑺𝒛𝒛 =𝑩𝑩+𝑬𝑬𝑴𝑴𝒛𝒛+𝑨𝑨𝝏𝝏 (11) where,

𝑩𝑩=−𝝆𝝆𝝆𝝆𝝆𝝆(𝒅𝒅 − 𝒅𝒅𝒐𝒐)

𝑬𝑬𝑴𝑴𝒛𝒛= 𝝁𝝁𝒆𝒆𝑰𝑰
𝟐𝟐
𝟒𝟒𝝅𝝅𝟐𝟐_{𝒓𝒓}𝟐𝟐_{𝒛𝒛}

𝑳𝑳�(𝟏𝟏 − 𝐞𝐞𝐞𝐞𝐞𝐞�− 𝒓𝒓𝟐𝟐 𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐��

𝟐𝟐
�_{𝒛𝒛}𝒛𝒛

𝑳𝑳�

𝑨𝑨𝝏𝝏=𝑪𝑪𝒍𝒍(𝟏𝟏−𝒇𝒇𝒍𝒍)

𝒇𝒇_{𝒍𝒍}𝟑𝟑+𝑪𝑪𝒔𝒔 𝝏𝝏 (12)
where the first two terms represents the momentum sources,
𝐵𝐵 as the buoyancy force, 𝐸𝐸𝐸𝐸𝑧𝑧 as the electromagnetic force
in the axial direction, these two terms were explained before.
The third momentum sink term is there to ensure that the
velocity disappears in solid cells and appears in liquid cells.
The determination of whether a cell would be solid or liquid
is by 𝑓𝑓𝑙𝑙 the liquid fraction; the two constants were chosen
deliberately to be 𝐶𝐶𝑙𝑙 large enough and 𝐶𝐶𝑠𝑠 small enough, to
avoid the division by 0 when the liquid fraction is 0 in the
solid. In the liquid zone, the sink term would fade away and a
velocity field is attained by the other momentum source
terms [26].

**Radial Momentum Source & Sink Term **

𝑺𝑺𝒓𝒓=𝑬𝑬𝑴𝑴𝒓𝒓+𝑨𝑨𝒓𝒓 (13) where,

𝑬𝑬𝑴𝑴𝒓𝒓= 𝝁𝝁𝒆𝒆𝑰𝑰 𝟐𝟐

𝟒𝟒𝝅𝝅𝟐𝟐_{𝝈𝝈}_{𝒋𝒋}𝟐𝟐𝒆𝒆𝒆𝒆𝒆𝒆 �−

𝒓𝒓𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐� �(𝟏𝟏 − 𝐞𝐞𝐞𝐞𝐞𝐞�−

𝒓𝒓𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐�� �

𝒛𝒛 𝒛𝒛𝑳𝑳�

𝟐𝟐

𝑨𝑨𝒓𝒓=𝑪𝑪𝒍𝒍(𝟏𝟏−𝒇𝒇𝒍𝒍)

𝒇𝒇_{𝒍𝒍}𝟑𝟑+𝑪𝑪𝒔𝒔 𝒓𝒓 (14)
where buoyancy force is no longer applicable in the
momentum source term, thus the source term would only
contain electromagnetic force which was explained in
Section x; and similarly, the momentum sink term would
take the same form as the one discussed in axial direction,
except the velocity is now in the radial direction 𝑢𝑢.

**Energy Source Term **

For a welding process, the energy source term would
account for the latent heat change during phase
transformation, in this case from solid to liquid. *Brent et al.*

[29] modelled the latent heat change as:

𝑺𝑺𝒆𝒆=− �𝝏𝝏𝝆𝝆∆𝑯𝑯_{𝝏𝝏𝝏𝝏} +𝛁𝛁 ∙(𝝆𝝆𝝆𝝆∆𝑯𝑯)� (15)
where ∆𝐻𝐻 is the enthalpy change and 𝑈𝑈 is the velocity

vector.

**Figure 9. ** Change of latent heat of fusion for pure metals (left); for alloyed
materials with the dashed line indicating the assumed linear profile (right)

The phase transformation for pure metals would occur
sharply at the melting temperature 𝑇𝑇𝑒𝑒; while at the same
time for alloyed materials, the phase change could happen
during an interval, from the solidus temperature 𝑇𝑇_{𝑠𝑠} to
liquidus temperature 𝑇𝑇𝑙𝑙 and the heat absorption is usually
non-linear as shown in Fig. 9 [27]. By assuming the change
of latent heat to be linear, some form of linearisation
technique is needed.

By iterating Eqn 15, Patankar [27], Voller & Swaminathan [28] were able to convert it into a linear equation:

𝑺𝑺𝒆𝒆=−𝝆𝝆𝑳𝑳𝝏𝝏𝒇𝒇_{𝝏𝝏𝒅𝒅}𝒍𝒍𝝏𝝏𝒅𝒅_{𝝏𝝏𝝏𝝏} (16)
The liquid fraction for alloyed materials would read:

𝒇𝒇𝒍𝒍=� 𝟎𝟎 𝒅𝒅−𝒅𝒅𝒔𝒔

𝒅𝒅_{𝒍𝒍−𝒅𝒅𝒔𝒔}
𝟏𝟏

𝒊𝒊𝒇𝒇 𝒅𝒅 ≤ 𝒅𝒅𝒔𝒔 𝒊𝒊𝒇𝒇 𝒅𝒅𝒔𝒔<𝒅𝒅<𝒅𝒅𝒍𝒍

𝒊𝒊𝒇𝒇 𝒅𝒅 ≥ 𝒅𝒅𝒍𝒍

(17)

where 𝑇𝑇𝑠𝑠 is the solidus temperature, 𝑇𝑇𝑙𝑙 the liquidus temperature and 𝐿𝐿 the latent heat of fusion.

**2.4. Velocity Boundary Conditions **

The velocity boundary condition is to be applied to the top surface, where surface tension temperature gradient would most definitely generate fluid flow not only on the weld pool surface, but also the pool interior.

**Top Surface by Marangoni Shear Stress **

Surface tension force would act in the tangential direction, and this force must be balanced by the viscous force subject to shear stress, the velocity boundary condition is therefore [19]:

−𝝁𝝁𝝏𝝏𝒓𝒓_{𝝏𝝏𝒛𝒛}=𝝏𝝏𝒅𝒅_{𝝏𝝏𝒅𝒅}∙𝝏𝝏𝒅𝒅_{𝝏𝝏𝒛𝒛} (18)
where 𝜇𝜇 is the viscosity of liquid metal and 𝑑𝑑𝛾𝛾/𝑑𝑑𝑇𝑇 is
worked as a single term to represent surface tension
temperature gradient.

**Effect of Surface Active Elements **

**2.5. Temperature Boundary Conditions **

The Temperature boundary conditions were divided into two categories: the heat source coming from the arc acting on the top surface and heat losses to the ambient environment on all surfaces. It can be expressed as:

𝒌𝒌 �𝝏𝝏𝒅𝒅_{𝝏𝝏𝒛𝒛}�=𝒒𝒒𝒊𝒊𝒊𝒊− 𝒒𝒒𝒐𝒐𝒓𝒓𝝏𝝏 (19)
where 𝑞𝑞𝑖𝑖𝑖𝑖 denotes the external arc heat source and 𝑞𝑞𝑜𝑜𝑜𝑜𝑜𝑜 as
the heat loss to the environment by radiation and convection
of surroundings.

**Arc Heat Source **

Only the top surface would experience external heat input, and this welding arc heat input could be modelled as

*Gaussian* heat distribution as [19]:

𝒒𝒒𝒊𝒊𝒊𝒊=_{𝟐𝟐𝝅𝝅𝝈𝝈}𝜼𝜼𝜼𝜼𝑰𝑰_{𝒋𝒋𝟐𝟐}𝒆𝒆𝒆𝒆𝒆𝒆 �− 𝒓𝒓

𝟐𝟐

𝟐𝟐𝝈𝝈𝒋𝒋𝟐𝟐� (20)

**Heat Losses **

All surfaces would be subject to convection and radiation heat transfer interacting with the ambient environment:

𝒒𝒒𝒐𝒐𝒓𝒓𝝏𝝏=𝒉𝒉𝒄𝒄(𝒅𝒅 − 𝒅𝒅𝑴𝑴) +𝝈𝝈𝒃𝒃𝜺𝜺(𝒅𝒅𝟒𝟒− 𝒅𝒅𝑴𝑴𝟒𝟒) (21)

where ℎ𝑐𝑐 is the convection heat transfer coefficient, 𝑇𝑇𝑎𝑎 is the ambient temperature, 𝜎𝜎𝑏𝑏 is the Stefan-Boltzmann constant and 𝜀𝜀 the emissivity of material.

**2.6. Software Implementation **

Meshing was refined towards the origin (*point A*) on both

*x* and *y* axes, these regions would be subject to intense heat
flux (temperature field initiation) as well as surface tension
effects (velocity field actuation), so that the model would
iterate more accurately initially from these crucial areas, and
the iterated results would be carried over to the succeeding
internal cells; if the starting calculations were not
comprehensive enough, then it would critically affect the
quality of the subsequent calculations.

**Figure 10. ** Schematic of workpiece and weld pool with reference axes

**Figure 12. ** Capture of the general meshing algorithm
Calculations to solve the velocity-pressure coupling was

handled by the SIMPLE convergence algorithm, an iteration process that pools the momentum and pressure in each time step, and gradually converging into the correct solution [27]. Moreover, the unique momentum and energy source terms were implemented and programmed into Fluent® as User-Defined Function (UDF), which was the core of the simulation programme.

**3. Model Validation **

**3.1. Enhancement Factor (EF) **

The use of enhancement factor was briefly outlined with respect to laminar or turbulent assumptions of the weld pool flow behaviour, in which whether the weld pool flow is laminar or turbulent is still not fully understood, even though reported literatures on weld pool simulations had been somewhat broadly studied. Nevertheless, enhancement factors were usually combined into the model to make up for underestimations on the momentum and energy calculations, and became the norm for welding simulations; so to get better agreement with the experimental results, regardless of the welding processes (GTAW, Laser welding, Electron Beam welding) [29]. This may be due to the fact that the flow process is confined to such a short time interval, yet also due to the highly unstable nature of the pool as well as plentiful forces acting on the welding pool that would further complicate the matter.

In short, the enhancement factor is applied to two material properties, liquid thermal conductivity and dynamic viscosity; these two terms were found to restrict the flow and alter weld pool geometries quite significantly (both width and depth) towards more desirable shapes compared to experimental data [8].

In this paper, the enhancement factor provides immediate and effective remedy in predicting the complex weld pool formation, but in a very primitive fashion with no clear guidelines.

Since the enhancement factor is utilised to cover for the lack of knowledge in the laminar or turbulence flow assumptions. Hong et al. [30] suggested that with a k-ε turbulent assumption, a maximum enhancement factor of 16 should be used for a stationary GTAW process (spot welding). This paper does somehow offer a general starting point for the simulations ran in this project, with simulation runs by enhancement factors in steps of 1(no enhancement), 2, 4, 8 and 16.

**Table 1. ** Operating conditions assumed in the reference case [31]

**3.2. Reference Case **

The reference case chosen to be evaluated against was by Pitscheneder et al. [31], where they studied the effect of sulphur content as surface active elements on the weld pool shape and liquid metal flow patterns. The reason for the selection is quite obvious, the paper had both experimental and simulation results, it was done under stationary arc conditions, and the effect of surface active elements in their model was also presented. Although it was under Laser welding, but the only difference in the physical model compared to GTAW would the absence of electromagnetic forces, hence the simulation was done with omission of this force accordingly. Strangely enough, the material used in the reference case was high speed steels, with varying level of sulphur concentrations; nonetheless, the material was implemented into the proposed model.

**3.3. Comparisons with Reference Case **

In the 1900 W scenario, Pitscheneder et al. [31] employed an enhancement factor of 4, and the proposed model had identical results when EF was set to 4. However, in both cases, the weld pool was slightly wider and shallower with their experimental results. If the power was adjusted up to 3850 W in the second scenario, good agreement with both the experimental and numerical results were gained, but with EF at 6 opposing to 7 used in the reference case. As for the 5200 W power setting scenario, the weld pool width is wider than the reference case, whereas the penetration conformed to the reference case quite well. Overall, the simulation results settled quite well with the reference case, this would permit confidence in the developed codes that is well validated for Marangoni driven welding simulations.

**4. GTAW Experiments **

Titanium alloy Ti-5Al-5Mo-5V-3Cr were spot welded in an incrementing time step of 1s for 5 steps for 40A; then starting at 0.5s, next from 1s to 5s in 1s time steps for 60A welds as shown in Fig. 14. Samples of metallography indicating the fusion zones are illustrated in Fig. 15.

**Figure 14. ** Ti-5Al-5Mo-5V-3Cr sample after spot welding of two current settings

**Figure 15.** Examples of Ti-5Al-5Mo-5V-3Cr fusion zone metallography; (a) 10V & 40A for 5 seconds; (b) 10V & 60A for 3 seconds.

**5. Simulation Result **

**5.1. Model Inputs & Associated Uncertainties **

**Table 3.** Key thermal properties of Ti-5Al-5Mo-5V-3Cr [32]

Stenbacka et al. [34] did a review of arc efficiency values used for up-to-date GTAW simulations, they found under direct current and negative electrode (DCEN) welding conditions, the arc efficiency values were between 36% and 90%; their study also suggested that with a 95% confidence, the arc efficiency for GTAW DCENwas approximated to be around 73 – 82%, or 78% in average. Thus the assumption for the welding efficiency for this model was based on their findings, with an estimated efficiency of 78%.

**Table 5.** Operating parameters of the simulations [34, 36]

The current distribution parameter (σj) on the other hand, is more troublesome since very small variations of this value would yield highly dissimilar results, and is often hardly practical to measure experimentally [35]. Saedi and Unkel [36] researched into the correlation between welding current and the current distribution parameter, their paper revealed a positive relationship between the two; as current increased,

the distribution parameter went up consequently. And according to their results, for a low current situation (40 – 60A), the current distribution parameter would sit around 1 mm, and therefore was assumed to be 0.8 mm at 40A and 1.2 mm at 60A.

Anyhow, without effective experimental and numerical procedures done to, e.g. arc efficiency, current distribution parameter and convective heat transfer coefficient etc. to model these parameters more accurately, the simulation results would contain considerable extent of uncertainties and seemingly biased.

**5.2. Sensitivity of Enhancement Factor **

Effect of EF on Weld Pool Geometry

First, by increasing the thermal conductivity and viscosity, the width of the pool saw a general declining trend regardless of the degree of surface tension temperature gradient. This may be due to increased viscosity; therefore there would be more resistance in flow movement.

**Figure 16.** Effect of EF on the pool geometry under 40A for 3s (a) width; (b) depth; (c) aspect ratio

**Effect of EF on Weld Pool Temperature **

Highest pool temperature was recorded when surface tension force was absent (at dγ⁄dT= 0), so much less convective heat transfer (high viscosity) which was replaced by high conductivity, or in another word heat is more focused at the pool centre. Since positive gradients would induce inward flows, this would also concentrate the heat to the centre, hence also producing high temperatures. Overall, with increasing enhancement factors, the maximum pool temperature declined, this would coincide with the general decreasing in pool size.

**5.3. Sensitivity of **𝒅𝒅𝒅𝒅/𝒅𝒅𝒅𝒅

Sensitivity analysis on the model was performed with varying degree of surface tension temperature gradients from -0.0005 to 0.0005 N/m∙K in steps of 0.0001 N/m∙K; its influence on the maximum weld pool temperature, maximum fluid velocity (negative being outward flow) and the weld pool aspect ratio were investigated as demonstrated in Fig. 18 & Fig.19.

**Effect of **𝒅𝒅𝒅𝒅/𝒅𝒅𝒅𝒅** on Weld Pool Geometry **

As one would expect, by varying the surface tension thermal gradient from negative to positive, the weld pool geometry went from wide and shallow to deep and narrow; also the width, depth and aspect ratio tends to increase/decrease in a linear pattern, without any critical points as seen in Fig. 18.

(a)

(b)

**Figure 18.** Influence of 𝜕𝜕𝛾𝛾 𝜕𝜕𝑇𝑇⁄ on the weld pool geometry: (a) size of
width and depth; (b) pool aspect ratio (D/W).

**Effect of **𝒅𝒅𝒅𝒅/𝒅𝒅𝒅𝒅** on Weld Pool Temperature & Flow **
**Velocity **

The weld pool temperature gradually increased as the surface tension thermal gradient moved towards zero, where the maximum temperature peaked usually high as seen in Fig. 19 (a). With absence of surface tension force, thermal mixing stimulating conductivity could not be fully utilised, instead localising the heat transfer inducing higher weld pool temperature and buoyancy force.

(b)

**Figure 19.** Variations of 𝜕𝜕𝛾𝛾 𝜕𝜕𝑇𝑇⁄ under 40A with respect to: (a) maximum
weld pool temperature; (b) maximum fluid velocity.

Furthermore, by examining the effect of surface tension temperature gradient on the flow velocities, interesting observations on the magnitude of the forces associated with the weld pool could be revealed. At ∂γ ∂⁄ T= 0, a very small negative (outward flow) velocity was usually induced, less than 2 cm/s in magnitude, reinforcing the theory that for GTAW process, surface tension forces would have the most profound impact; the outward flow direction suggests that buoyancy forces (outward flow) would outweigh electromagnetic force (inward flow), since these are the only two forces existing in this model. Moreover, the velocity magnitudes for positive gradients are much larger than when negative, this may be due to the fact that gravitational force would stimulate the inward flow, further speeding up the circulating flow initiated from the top surface.

**6. Comparison of Results **

**6.1. Flow Regime **

**Figure 20. ** Comparison of results between (a) laminar flow scheme; (b)
original turbulent flow assumption; under 60A power for 0.5 seconds & EF
= 2 & dγ⁄dT=-0.00042 N/m∙K

As explained in introduction, the laminar or turbulent assumption has always been at the centre of numerical welding researches, and for past studies, researchers had assumed the pool to be either consistently laminar or turbulent, with no crossovers of these two; Whereas this time, the model was converted based on laminar flow assumptions at shorter welding times, and saw the breakthrough in predicted weld pool geometry.

Under the 60A power setting, with a 𝑘𝑘 − 𝜀𝜀 turbulent assumption, the weld pool would not even appear if the welding time was set to 0.5s, as shown in Fig. 20 (b). On the other hand, with a laminar flow setup, the model was able to produce “bang on” predictions of the overall weld pool shape.

Having proved that during the early stages of the weld pool formation, laminar flow assumption would be more appropriate, but there must be a period of transition to turbulent flow. Fig. 21 is illustrating the results under the same 60A welding current, with time progressed to 2 seconds, none of which had brilliant match with the experimental results. The laminar assumption was over predicting the weld pool shape; hence the stream had already gone past the laminar flow guess. At the same time, turbulent assumption would under calculate the pool size by a large fraction. These combined would imply that the pool at the 2-second instant is probably undergoing laminar to turbulent transition, thus no viable match could be realised given keeping all else constant.

**Figure 21. ** Comparison of results between (a) laminar flow scheme; (b)
original turbulent flow assumption; under 60A power for 2 seconds; EF = 2
& dγ⁄dT=-0.00042 N/m∙K

**Figure 22.** Good agreement of overall pool shape with turbulent flow
regime; under 60A for 3 seconds; at EF = 2 & dγ⁄dT=-0.00042 N/m∙K

**6.2. Estimation of **𝒅𝒅𝒅𝒅/𝒅𝒅𝒅𝒅** and ****EF**** for **
**Ti-5Al-5Mo-5V-3Cr **

As for the current study, the weld pool shape had a good agreement with an enhancement factor of 2, negative surface tension temperature gradients was also discovered with slight variations for the two power settings, −0.00035 𝑁𝑁/ 𝑚𝑚 ∙ 𝐾𝐾 for the 40A case and −0.00042 𝑁𝑁/𝑚𝑚 ∙ 𝐾𝐾 under the 60A scenario.

**7. Conclusions **

A simulation model of GTAW process has been developed in this paper to investigate the weld pool shape variations due to Marangoni effect and surface tension shear stress. Based on the results, by enhancing the liquid thermal conductivity and viscosity simultaneously, the weld pool size shrank, so does the pool temperature and flow velocity, suggesting the added resistance to flow by viscosity would object the heat transfer more than conductivity, confirming the weld pool shape would be more sensitive to changes in viscosity than thermal conductivity, reinforcing convective heat transfer would be more significant than conductive heat transfer.

By varying the dγ⁄dT value from negative to positive, the weld pool geometry went from wide and shallow to deep and narrow; the pool width, depth, and aspect ratio tend to increase/decrease linearly with no critical points for Ti-5Al-5Mo-5V-3Cr. With the absence of Marangoni Effect (dγ⁄dT= 0), a tiny negative (outward flow) velocity vector was present, made up by buoyancy effect (outward flow) and electromagnetic force (inward flow); this would settle that Marangoni Effect being the most dominant force in shaping the weld pool, followed by buoyancy effect and electromagnetic force under the GTAW process. Titanium alloy Ti-5Al-5Mo-5V-3Cr under investigation was found to constitute high negative ∂γ ∂⁄ T values during GTAW process, overall good agreement of simulation results to experimental data was obtained by a relatively low enhancement factor of 2.

**Acknowledgements **

This work was sponsored by School of Engineering, Auckland University of Technology, New Zealand.

**REFERENCES **

[1] DebRoy, T. & David, S.A., (1995). Physical processes in fusion welding. Reviews of Modern Physics. Vol.67, Issue 1, p85-112.

[2] Limmaneevichitr, C., (2000). Flow visualization of Marangoni convection in simulated weld pools. Ph.D. dissertation. University of Wiscousin-Madison, USA. [3] Katayama, S. et al., (2001). X-ray transmission in-situ

observation of fluid flow inside molten pool during tig arc welding of stainless steel. Transactions of JWRI. Special Issue: 3rd International Conference of High Temperature Capillarity 2000. Vol.30.

[4] Berthier, A., Paillard, P., Carin, M., Valensi, F., Pellerin, S.
(2012) TIG and a-TIG welding experimental investigations
and comparison to simulation part 1: Identification of
Marangoni effect. *Science and Technology of Welding and *
*Joining 17(8): 609-615. *

[5] Xia, D., Xu, B.-S., Lv, Y.-H., Yi, J., Liu, C.-L. (2012) Effect
of Marangoni convection on welding pool of plasma direct
metal forming finite element model. *Materials Science *
*Forum 704-705: 674-679. *

[6] Sándor, T., Mekler, C., Dobránszky, J., Kaptay, G. (2013)
An improved theoretical model for A-TIG welding based on
surface phase transition and reversed Marangoni flow.
*Metallurgical and Materials Transactions A: Physical *
*Metallurgy and Materials Science 44(1): 351-361. *

[7] Traidia, A., Roger, F. & Guyot, E., (2010). Optimal parameters for pulsed gas tungsten arc welding in partially and fully penetrated weld pools. International Journal of Thermal Science. Vol.49, Issue 7, p1197-1208.

[8] De, A. & DebRoy, T., (2004). A smart model to estimate effective thermal conductivity and viscosity in the weld pool. Journal of Applied Physics. Vol.95, Issue 9, p5230-5240. [9] Vowell, S., (2009). Microfluids: the effects of surface

tension. Physics department, University of Washington, USA.

[10] Bragard, J. & Velarde, M.G., (1998). Benard-Marangoni convection: planforms and related theoretical predictions. Journal of Fluid Mechanics. Vol.368, p165-194.

[11] Ehlen, G., Ludwig, A. & Sahm, P.R., (2003). Simulation of Time-dependent pool shape during laser spot welding: transient effects. Metallurgical and Materials Transactions A. Vol.34A, p2947-2961.

[12] Aidun, D. & Martin, S., (1997). Effect of sulphur and oxygen on weld penetration of high-purity autenitic stainless steels. Journal of Materials Engineering and Performance. Vol.6, p496-502.

the shape of the gta, laser and electron beam welds. Welding Journal. Vol.62, Issue 3, p72.

[14] Limmaneevichitr, C. & Kou, S., (2000). Experiments to simulate effect of Marangoni convection on weld pool shape. Welding Research Supplement. P231-237.

[15] Sahoo, P., DebRoy, T. & McNallan, M., (1988). Surface tension of binary metal – surface active solute systems under conditions relevant to welding metallurgy. Metallurgical Transactions B. Vol.19, p483-491.

[16] Kou, S. & Sun, D.K., (1985). Fluid flow and weld penetration in stationary arc welds. Metallurgical Transaction A. Vol.16A, Issue 2, p203-213.

[17] Kou, S. & Wang, Y.H., (1986). Weld pool convection and its effect. Welding Journal. Vol.65, Issue 3, p63-70.

[18] Kumar, A. & DebRoy, T., (2005). Tailoring complex weld geometry through reliable heat transfer and fluid flow caluclations and a genetic algorithm. Metallurgical and Materials Transactions A. Vol.36A, p2725-2735.

[19] ] Shi, Y. et al., (2011). Numerical simulation of the force in TIG welding pool based on Fluent. Electric Welding Machine. Vol.41, Issue 9, p21-24.

[20] Kou, S., (1987). Welding metallurgy. New York: Wiley. [21] Lee, H.G. & Kim, J., (2012). A comparison study of the

Boussinesq and the variable density models on buoyancy-driven flows. Journal of Engineering Mathematics. Vol.75, Issue 1, p15-27.

[22] Lin, M.L. & Eagar, T.W., (1986). Pressures produced by gas tungsten arcs. Metallurgical Transactions B. Vol.17B, p601-607.

[23] Choo, T.C. & Szekely, J. (1991). The effect of gas shear stress on Marangoni flows in arc welding. Welding Research Supplement. P223-233.

[24] Matsunawa, A. & Yokoya, S., (1989). Fluid flow and its effect on penetration shape in stationary arc welds. Recent Trends in Welding Science and Technology. Proceedings from 2nd International Conference, Gatlinburg. ASM International.

[25] Fluent® Tutorial Guide. ANSYS®. 2009.

[26] Brent, A., Voller, V. & Reid, K., (1988). Enthalpy-porosity technique for modelling convection-diffusion phase change: application to the melting of pure metal. Numerical Heat Transfer B. Vol.13, p297-318.

[27] Patankar, S.V., (1980). Numerical heat transfer and fluid flow. Hemisphere, New York, USA.

[28] Voller, V.R., & Swaminathan, C.R., (1991). General source-based method for solidification phase change. Numerical Heat Transfer Part B Fundamentals. Vol.19, Issue 2, p175-189.

[29] De, A. & DebRoy, T., (2005). Reliable calculations of heat and fluid flow during conduction mode laser welding through optimization of uncertain parameters. Welding Journal. Vol.84, Issue 7, p101-112.

[30] Hong, K. et al., (2002). Modelling turbulent thermofluid flow in stationary gas tungsten arc weld pools. Science and Technology of Welding and Joining. Vol.7, Issue 3, p125-136.

[31] Pitscheneder, W. et al., (1996). Role of sulphur and processing variables on the temporal evolution of weld pool geometry during multi-kilowatt laser beam welding of steels. Supplement to the Welding Journal. p71.

[32] Luo, L. et al, (2009). Brief introduction for BT22 titanium alloy. Journal of Hot Working Technology. Vol.38, Issue 14, p14-16.

[33] Department of Physical Engineering, Marochnik. (2013). Database of Steel and Alloy: VT22. Retrieve on 19 Aug 2013 from:

http://www.splav.kharkov.com/en/e_mat_start.php?name_id =1302

[34] Stenbacka, N., Choquet, I. & Hurtig, K., (2012). Review of arc efficiency values for gas tungsten arc welding. Intermediate Meeting BAM.

[35] Pierce, S.W., Burgardt, P. & Olsen, D.L., (1999). Thermocapillary and arc phenomena in stainless steel welding. Welding Research Supplement, p45-52.